# , to obtain a way to calculate stress from the energy function U(r).

Size: px
Start display at page:

Download ", to obtain a way to calculate stress from the energy function U(r)."

## Transcription

1 BIOEN LECTURE : MOLECULAR BASIS OF ELASTICITY Estimating Young s Modulus from Bond Energies and Structures First we consider solids, which include mostly nonbiological materials, such as metals, plastics, ceramics, and covalently bound solids like diamonds. We will consider the molecular structure of these materials and how this determines the materials properties. First, we learn to estimate the Young s modulus of these materials from the molecular structure, which determines their behavior at sufficiently small deformations. Next we ask what happens when we deform them beyond the point where the stress-strain relationship becomes nonlinear, meaning the ratio of stress to strain is no longer constant and the Young s modulus no longer applies. Only mechanical testing experiments can provide the exact Young s modulus of a material, but one can estimate the Young s modulus from knowledge about the molecular structure of the material. This is useful when designing a material, determining the right mechanical test for a material, or simply understanding materials properties better. In general, materials are made up of atoms or molecules, which we call nodes for the purposes of this discussion, and these interact with each other through what we call bonds. For diamond, the nodes are the carbon atoms, and the bonds are the covalent bonds between carbon atoms. For a collagen scaffold, a node is where two fibers are cross-linked, and the bond is the length of fiber between two cross-links. Consider now an idealized material that has the nodes in a square matrix as in Figure 1. Let r 0 be the equilibrium bond length in unstressed material. What do stress, strain, and the Young s modulus mean on the nanoscale level of single bonds? If we apply a stress, σ, to the material, how much force is applied to each bond? Consider a single bond that is Figure 1. Idealized material parallel to the direction of force. How is it spaced from the bonds that are parallel to it? Because the matrix is square, each node and thus bond has a cross-sectional area of r 0, so structure geometry. with cubic node the force per bond is f = r 0 σ. We also remember what we learned last lecture: f = du, to obtain dr a way to calculate stress from the energy function U(r). σ = f du r = dr (r) 0 r 0 Next we ask if the resulting strain on the material is ε, then how much does each bond stretch? The original bond length is r 0, so it stretches r r 0 = Δr = r 0 ε by the definition of strain. Thus, ε = Δr = r r 0 r 0 r 0 We can combine this to relate stress to strain using the energy function. That is, if we know U(r), then we calculate the value at which this is minimum to get r 0, and then can calculate both stress and strain for any bond length r. The ratio is of particular interest: 1

2 σ ε = f r 0 r 0 Δr = f r 0 (r r 0 ) = du dr (r) r 0 (r r 0 ) Depending on the Energy function, this may not be a linear relationship. However, for sufficiently small deformations, we can use the linear approximation: f = du = k(r r dr 0), where k = d U (r dt 0). For these small deformations, σ ε = k(r r 0) r 0 (r r 0 ) = k d U = dr (r 0) r 0 r 0 This is a constant relationship between stress and strain, and thus is the Young s modulus: E = k d U = dr (r 0) r 0 r 0 Thus, we can use the full version of the energy function to relate stress to strain, and can use the linear spring form to estimate the Young s modulus. Limitations: If a material is stretched so that the bonds are stretched beyond the linear spring approximation, the linear approximation will not be valid, and the material will show nonlinear properties and eventually fail. This derivation assumed that the material was a perfect square lattice, but most materials have different crystalline lattices or even noncrystalline Figure. Other bond-node geometries affect these calculations. lattices. This introduces some error to our calculation. The area may not be exactly r 0, and bonds may be angled relative to the direction of force. Indeed, the material may stretch as bond angles change as well as when bond length increases, as in Figure. This derivation also assumed that all bonds were the same. In fact, many materials, especially biological materials, have many different types of bonds. In this case, the weakest of the bonds is the primary determinant of the Young s modulus, just as the stiffness of springs in parallel is dominated by the softest springs. Thus, for mixed materials, we consider the mean length between the softer bonds. Molecular Structure and Elasticity of Various Solids Now we will consider the different types of bonds that make up materials, and learn their energy functions and typical parameters of these functions so we can estimate the Young s modulus.

3 Covalent solids: Covalent solids are held together by covalent bonds. Covalent bond energy is approximated by a spring, with U(r) = 1 k(r r 0), where k is the spring constant of the bond. Since this bond energy is already a linear spring form, we obtain the same answer if we use the linear approximation or full function: E = k/r 0. An example of a covalent solid is a diamond in which carbon atoms form a tetrahedryl lattice. For a typical Figure 3. Covalent Bond energy covalent solid, k = 150 N/m and r 0 = 1.5e 10 m. Thus, E 10 1 N/m. Note that 10 9 N/m = 1 GPa, so we would expect a covalent solid to have a Young s modulus of around 1000 GPa. In fact, diamond has a modulus of E = 100 GPa, so this estimate is good. Metallic solids. In metals, the electrons in the outer valence shells are shared by many atoms and thus are delocalized. Thus, while the atoms still form regular crystal structures like covalent solids, they tolerate irregularities so that the overall structure is more disordered. The bond stiffness in metallic solids is weaker than covalent, at about N/m, so the Young s moduli of metals are several fold weaker than for covalent solids. Ionic solids Ionic solids include salts like NaCl and ceramics like ZrO (zirconia), Alumina, and hydroxyappetite, which forms the inorganic part of bone. The crystalline structures of these solids have alternating positive and negative ions. The bond force between each pair is a complicated sum of the following forces: Figure 4. Ionic Solid The attractive force between that pair, which is U = q 1q 1, where q 4πε 0 ε r r 1 and q are the charges of the two ions (e.g. 1.6e-19 C for Na), ε 0 = 8.3e 1 C Nm is the permittivity of free space, ε r = 6 is the dielectric constant of typical salts. The van der Waals repulsion between that pair of atoms The sum of attractive and repulsive forces of neighboring atoms, which are significant for quite some distance since they only drop with the inverse of the distance. Calculating these forces from the information above is beyond the scope of this class, but in general, ionic bonds stiffnesses are known to be around 8 to 4 N/m and bond lengths are also longer than in covalent or metallic bonds, so salts are much softer. For example, the Young s modulus of NaCl is 40 GPa. 3

4 Van der Waal s solids Finally, consider a van der Waal s solid, such as a hard plastic. These materials are made up of polymers that have many intramolecular covalent bonds, but these interact through intramolecular and intermolecular van der Waal s (VDW) bonds. As we will see below, the VDW bonds are weaker than the covalent bonds, so they determine the Young s modulus of VDW solids such as hard plastic. The Lennard Jones Potential approximates VDW energies: U(r) = U 0 r 0 r 1 r 0 r 6, Here, r 0 = r i + r j is the sum of the VDW radii of the two atom types. U 0 = U i U j, where U i is the bond energy for atom type i. For example, a N-C bond would have r 0 = = 3.5Å and U 0 = 4.7E 7.E = 5.8E J. While energy estimates vary by method and covelent connections, the table to the right provides values for some atom types for r i and U i. Note from the equation and the figure that: U(0) = U 0 ( 1 6 ) = U(r 0 ) = U 0 (1 ) = U 0 U( ) = U 0 (0 0) = 0 In the homework, you will show that VDW solids have Young s moduli of a few GPa. Proteins are polypeptides, which are covalent polymers, but fold up into alpha helices and beta sheets, that are held together by hydrogen bonds. Finally, these secondary structure elements are held together by VDW interactions, at least in globular proteins. The VDW interactions are the softest of these, so globular proteins have a Young s modulus of a few GPa, and are fairly isotropic. For examples, the Young s modulus of microtubules and actin filaments have both been measured at around GPa. However, proteins are not always globular, and can thus have a wide range of behaviors. We will consider many of these in the next few lectures. Hydrogels Element radius (Å) energy (J) H E- C E- N E- O E- Like plastics, hydrogels are made up of polymers. However, the polymers are hydrophilic and soak up water. We learned before that water causes viscosity in these materials. The presence of water between the polymers also prevents most of the intramolecular and intermolecular van der Waals bonding, so a mixture of these hydrophilic polymers would form a viscous liquid instead of a hard plastic. Cross-linking between the polymers creates nodes, so the polymers form bonds that can be addressed quantitatively as described above. Hydrogels are often very soft relative to other surfaces, and can tolerate large strains, even greater than 1. The next lectures will address the nonlinear behaviors that often arise for hydrogels, including biological tissues. 4

5 Nonlinear Materials Properties. Review of Nonlinear Materials Properties and Failure Hooke s law (σ = Eε) applies below a critical point called the proportional limit characterized by the stress and strain at this point: σ PL and ε PL. Above the proportional limit, the stress-strain relationship becomes nonlinear, meaning the ratio of stress to strain is no longer constant, but either increases or decreases with further stress or strain. For some materials, the proportional limit is clearly defined, while for others, the boundary is less clear and can only be identified after defining an allowable deviation from linearity. In the nonlinear regime above the proportional limit, we cannot define a Young s Modulus, since by definition that requires a constant ratio of stress to strain. Instead, we define the tangent Young s modulus as the slope of the stress/strain curve: E T = dσ/dε. If the tangent Young s modulus decreases with strain (d σ/dε < 0), we refer to this as yielding. If the tangent Young s modulus increases with strain (d σ/dε < 0), we refer to this as strain hardening. Below a critical point called the elastic limit, the material relaxes back exactly to its original shape when force is removed. The elastic recovery occurs because the bonds described above never break within this limit, but instead are simply stretched, so return to the original low-energy position in the absence of force, which is the equilibrium bond length. Usually, all deformations below the proportional limit are elastic, so one can usually guaranteed that the material is undamaged as long as the stress is still proportional to the strain during loading. If a material is stretched beyond a critical point, the atomic or molecular bonds break. For covalent solids, metals, plastics and ceramics (the materials we discussed on Friday), this occurs at about the proportional limit; that is, the bonds break shortly beyond the point where they are stretched beyond the linear range. We will see that this is not the case for most gels and soft and biological materials. For ductile materials, bonds can reform between two atoms or molecules that were not previously bonded. In this case, the material deforms substantially beyond the proportional limit. But, when the force is removed, it will not return to its original shape, since the molecular bonds have reformed into new connections that determine the shape. 5

6 The fractional change in length after stress is removed is called residual strain. Irreversible deformation like this is referred to as plastic deformation. However, as the plastically deformed material is relaxed, there is a small amount of elastic recovery as the bonds return to their equilibrium length. However, due generally in the amount expected from the proportional limit. The yield point (characterized by yield stress σ Y and yield strain ε Y ), is the point between the elastic and plastic regime. While the proportional limit can be identified while increasing the load on a material, the yield point can only be identified when the load is added and then removed. Thus, a material is repeatedly stretched and relaxed to increasingly greater strains to identify the yield point. The exact yield point is impossible to identify due to errors in measurements, so by convention, it is approximated by the elastic limit, which is defined as the stress and strain that will cause a permanent 0.% deformation in the material upon relaxation. If the relaxed material is now stressed again below the yield point, it behaves elastically. For brittle materials, the rupture of bonds causes the material to fracture, or break catastrophically along the points of most stress. In brittle materials, bonds do not readily reform, so the material fails completely when the original bonds are overstretched. Even ductile materials will fracture eventually, as the material is deformed in some way that does not allow bonds to reform. The maximum stress σ MAX is the highest stress the material can withstand prior to fracture. Because some materials may reduce the strain prior to fracture, the maximum stress is not necessarily the stress at fracture. The breaking strain ε MAX is the strain at fracture. The tensile strength of a material is σ MAX during tension, while the compressive strength is σ MAX for compression. These are often not the same. Molecular Basis of Plastic Deformation and Failure Above the proportional limit, different materials behavior very differently in terms of whether they yield or strain harden and where they fracture relative to their elastic limit (brittle vs ductile). Thus, we now consider specific materials. Note that you can calculate the strain at the proportional limit by dividing the yield stress or by the Young s modulus, since the material are generally linear before they yield. Metals The shared electrons in metal atoms allows bonds to easily break and reform so that the material can rearrange along slip planes when exposed to shear stress: 6

7 Metals are usually polycrystalline, with many small regions that are crystalline and regular, but each small region is oriented randomly, which is why the crystalline materials is still isotropic. The stress needed to cause a small region to slip depends on its orientation relative to the stress, so that only a few ideally oriented ones slip at the plastic limit (yield point), but more and more slip as stress increases higher. Because of this, the stress-strain curve gradually slopes for typical metals: To understand how much deformation is allowed before slippage, note that the yeild stress of aluminum is 95 MPa, while the Young s modulus is 69 GPa, so the yield strain is about 95E6/69E9 ~ 0.1%. For stainless steel, the value is 180 GPa and 50 MPa, or 0.3%. Thus, metals can only deform by 0.1% to 0.3% before they undergo plastic deformation, but do not fracture because they are ductile. Ceramics. In contrast, ceramics are generally resistant to slip along planes because of the electrostatic interactions. They also leave the proportional limit at about 0.1 to 0.3% strain. However, the resistance to slip means they are brittle and fracture when the bonds break. Some polymers are also brittle. Amorphous polymers. Most polymers are amorphous, with the covalently bonded polymers oriented randomly, and interactions within and between chains are primarily VDW interactions. Because VDW interactions are long range and packing is noncrystalline, the polymers can slide along each other, alowing yielding. The yielding is plastic because the VDW bonds have broken and 7

8 reformed. Finally, because there is no crystaline organization, the orientation of the stress to the material doesn t matter like in metals, so the material continues to deform at the yield stress. Thus, the stress-strain curve flattens out and the tangent Young s modulus becomes nearly zero. Nevertheless, above some point, the polymers become aligned in a way that limits further slipping, which causes the plastic to exhibit strain hardening. However, as the material continues to stretch, the cross-section gets smaller due to the lateral strain. At sufficiently large deformations, this effect cannot be ignored. The true stress is the force divided by the actual cross-sectional area measured at that force. However, most graphs, including that above, display the engineering stress, which is defined to be the force applied divided by the original unstressed cross-sectional area. The engineering stress represents the direct measurement in a tensile test, without needing to measure the cross-sectional area at each point. It also can predict how a object will behave in an engineering application. As the crosssectional area decreases, and the material is already yielding, the true stress will stay the same but the engineering stress will drop as shown in the sketch above, due to the ever smaller crosssection. In an engineering situation, this drop leads to catastrophic failure as the member supports less and less stress. As for all materials, sufficient stress and strain will eventually cause fracture. Polymers typically have a much higher yield strain than do ceramics or metals, allowing 1 to 3% strain. 8

### Lösungen Übung Verformung

Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress- strain diagram? 2. Name the four main

### Materials Issues in Fatigue and Fracture

Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view

### EUROLAB 25 years. The role of metrology and testing to characterize materials and products. EUROLAB 25th Anniversary Seminar

EUROLAB 25 years The role of metrology and testing to characterize materials and products April 9, 2015, Odense Danmark 1 Origin of Conformity Assessment The New Approach for the European Economic Community

### Unit 11 Practice. Name: Class: Date: Multiple Choice Identify the choice that best completes the statement or answers the question.

Name: Class: Date: Unit 11 Practice Multiple Choice Identify the choice that best completes the statement or answers the question. 1) Crystalline solids. A) have their particles arranged randomly B) have

### CARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES

26 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES CARBON/DYNEEMA INTRALAMINAR HYBRIDS: NEW STRATEGY TO INCREASE IMPACT RESISTANCE OR DECREASE MASS OF CARBON FIBER COMPOSITES J. G. H. Bouwmeester*,

### Tensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density

Engineering Solid Mechanics 3 (2015) 35-42 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens

### Polymer Melt Rheology. Introduction to Viscoelastic Behavior. Time-Temperature Equivalence

Topics to be Covered Polymer Melt Rheology Introduction to Viscoelastic Behavior Time-Temperature Equivalence Chapter 11 in CD (Polymer Science and Engineering) Polymer Melt Rheology δ τ xy Newton s Law

### ME 612 Metal Forming and Theory of Plasticity. 1. Introduction

Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations

### Chapter 8 Maxwell relations and measurable properties

Chapter 8 Maxwell relations and measurable properties 8.1 Maxwell relations Other thermodynamic potentials emerging from Legendre transforms allow us to switch independent variables and give rise to alternate

### SEISMIC UPGRADE OF OAK STREET BRIDGE WITH GFRP

13 th World Conference on Earthquake Engineering Vancouver, B.C., Canada August 1-6, 2004 Paper No. 3279 SEISMIC UPGRADE OF OAK STREET BRIDGE WITH GFRP Yuming DING 1, Bruce HAMERSLEY 2 SUMMARY Vancouver

### B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS

B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions

### Chapter 7: Polarization

Chapter 7: Polarization Joaquín Bernal Méndez Group 4 1 Index Introduction Polarization Vector The Electric Displacement Vector Constitutive Laws: Linear Dielectrics Energy in Dielectric Systems Forces

### ITU Department of Mechanical Engineering. MANUFACTURING PROPERTIES of ENGINEERING MATERIALS Lecture Notes. Prof.Dr.Ahmet Aran

ITU Department of Mechanical Engineering MANUFACTURING PROPERTIES of ENGINEERING MATERIALS Lecture Notes Prof.Dr.Ahmet Aran 2007 CONTENTS 1. Engineering Materials and Their Properties 1.1. Classification

### Part B 2. Allow a total of 15 credits for this part. The student must answer all questions in this part.

Part B 2 Allow a total of 15 credits for this part. The student must answer all questions in this part. 51 [1] Allow 1 credit for 3 Mg(s) N 2 (g) Mg 3 N 2 (s). Allow credit even if the coefficient 1 is

### Underwater Tablet Enclosure Final Report by Miguel de Villa

Underwater Tablet Enclosure Final Report by Miguel de Villa Abstract: The underwater tablet enclosure is a device used to maximize the protection and survivability of a tablet underwater without losing

### 1. When we deform a material and it recovers its original shape, we say that it is a) Rigid

UNIT 05 TEST TECHNOLOGY 1º ESO GROUP: A DATE: / / 1. When we deform a material and it recovers its original shape, we say that it is 2. When we try to deform a material and it doesn t change its shape,

### EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL

EFFECT OF SEVERE PLASTIC DEFORMATION ON STRUCTURE AND PROPERTIES OF AUSTENITIC AISI 316 GRADE STEEL Ladislav KANDER a, Miroslav GREGER b a MATERIÁLOVÝ A METALURGICKÝ VÝZKUM, s.r.o., Ostrava, Czech Republic,

### Dynamics in nanoworlds

Dynamics in nanoworlds Interplay of energy, diffusion and friction in (sub)cellular world 1 NB Queste diapositive sono state preparate per il corso di Biofisica tenuto dal Dr. Attilio V. Vargiu presso

### 2.5 Physically-based Animation

2.5 Physically-based Animation 320491: Advanced Graphics - Chapter 2 74 Physically-based animation Morphing allowed us to animate between two known states. Typically, only one state of an object is known.

### Chapter Outline: Phase Transformations in Metals

Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations

### TENSILE BEHAVIOUR OF OPEN CELL CERAMIC FOAMS

Original papers TENSILE BEHAVIOUR OF OPEN CELL CERAMIC FOAMS LUKÁŠ ŘEHOŘEK*, **, IVO DLOUHÝ*,**, ZDENĚK CHLUP* *Institute of Physics of Materials ASCR, Žižkova 22, 616 62 Brno, Czech Republic **Institute

### Applied virtual (VT) technology on bus superstructure roll-over tests

Applied virtual (VT) technology on bus superstructure roll-over tests VINCZE-PAP Sándor 1, CSISZÁR András 2 1 JÁFI-AUTÓKUT Engineering Ltd., H-1115 Budapest, Csóka u. 7-13., email: vincze_pap@jafi-autokut.hu

### Introduction to Tensile Testing

CHAPTER 1 Introduction to Tensile Testing TENSILE TESTS are performed for several reasons. The results of tensile tests are used in selecting materials for engineering applications. Tensile properties

### Investigation of a Macromechanical Approach to Analyzing Triaxially-Braided Polymer Composites

NASA/TM 2010-216371 AIAA 2010 2522 Investigation of a Macromechanical Approach to Analyzing Triaxially-Braided Polymer Composites Robert K. Goldberg Glenn Research Center, Cleveland, Ohio Brina J. Blinzler

### 5. MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS

5. MECHANICAL PROPERTIES AND PERFORMANCE OF MATERIALS Samples of engineering materials are subjected to a wide variety of mechanical tests to measure their strength, elastic constants, and other material

### Chapter 4. Electrostatic Fields in Matter

Chapter 4. Electrostatic Fields in Matter 4.1. Polarization A neutral atom, placed in an external electric field, will experience no net force. However, even though the atom as a whole is neutral, the

### Precision Miniature Load Cell. Models 8431, 8432 with Overload Protection

w Technical Product Information Precision Miniature Load Cell with Overload Protection 1. Introduction The load cells in the model 8431 and 8432 series are primarily designed for the measurement of force

### Modern Codes for Design of Concrete Concrete Structures Presentation Outline

Modern Codes for Design of Concrete Structures James K. Wight F.E. Richart, Jr. Professor of Civil Eng. University of Michigan Presentation Outline Current Codes Where did they come from? What is their

### Hands-on exercises on solvent models & electrostatics EMBnet - Molecular Modeling Course 2005

Hands-on exercises on solvent models & electrostatics EMBnet - Molecular Modeling Course 2005 Exercise 1. The purpose of this exercise is to color the solvent accessible surface of a protein according

### Practice Final Math 122 Spring 12 Instructor: Jeff Lang

Practice Final Math Spring Instructor: Jeff Lang. Find the limit of the sequence a n = ln (n 5) ln (3n + 8). A) ln ( ) 3 B) ln C) ln ( ) 3 D) does not exist. Find the limit of the sequence a n = (ln n)6

### BEHAVIOR OF WELDED T-STUBS SUBJECTED TO TENSILE LOADS

BEHAVIOR OF WELDED T-STUBS SUBJECTED TO TENSILE LOADS R.A. Herrera 1, G. Desjouis 2, G. Gomez 2, M. Sarrazin 3 1 Assistant Professor, Dept. of Civil Engineering, University of Chile, Santiago, Chile 2

### Chemistry 201. Practical aspects of buffers. NC State University. Lecture 15

Chemistry 201 Lecture 15 Practical aspects of buffers NC State University The everyday ph scale To review what ph means in practice, we consider the ph of everyday substances that we know from experience.

### Types of Strain. Engineering Strain: e = l l o. Shear Strain: γ = a b

Types of Strain l a g Engineering Strain: l o l o l b e = l l o l o (a) (b) (c) Shear Strain: FIGURE 2.1 Types of strain. (a) Tensile. (b) Compressive. (c) Shear. All deformation processes in manufacturing

### Estimation of shear force for blind shear ram blowout preventers

Estimation of shear force for blind shear ram blowout preventers Abdulkadir Tekin *, Changhyok Choi, Taylan Altan, Hamit Adin Online Publication Date: 17 Feb 2015 URL: http://www.jresm.org/archive/resm2014.02st1225.html

### Exam 1 Sample Question SOLUTIONS. y = 2x

Exam Sample Question SOLUTIONS. Eliminate the parameter to find a Cartesian equation for the curve: x e t, y e t. SOLUTION: You might look at the coordinates and notice that If you don t see it, we can

### Modelling of Contact Problems of Rough Surfaces

Modelling of Contact Problems of Rough Surfaces N. Schwarzer, Saxonian Institute of Surface Mechanics, Am Lauchberg 2, 04838 Eilenburg, Germany, Tel. ++49 (0) 3423 656639 or 58, Fax. ++49 (0) 3423 656666,

### ABSTRACT 1. INTRODUCTION 2. DESCRIPTION OF THE SEGMENTAL BEAM

Ninth LACCEI Latin American and Caribbean Conference (LACCEI 11), Engineering for a Smart Planet, Innovation, Information Technology and Computational Tools for Sustainable Development, August 3-, 11,

### Module 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV

Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &

### Analysis of Bolted Connections in Creo Simulate - Theory, Software Functionality and Application Examples -

Analysis of Bolted Connections in Creo Simulate - Theory, Software Functionality and Application Examples - Dr.-Ing. Roland Jakel, Altran Aviation Engineering 5 th SAXSIM, TU Chemnitz Rev. 1.1 April 23

### COMPOSITE MATERIALS. Asst. Prof. Dr. Ayşe KALEMTAŞ

COMPOSITE MATERIALS Office Hours: Tuesday, 16:30-17:30 akalemtas@mu.edu.tr, akalemtas@gmail.com Phone: +90 252 211 19 17 Metallurgical and Materials Engineering Department CONTENT Composite Materials Metal

### When to Use Immediate Settlement in Settle 3D

When to Use Immediate Settlement in Settle 3D Most engineers agree that settlement is made up of three components: immediate, primary consolidation and secondary consolidation (or creep). Most engineers

### Inside Hair: A Closer Look at Color and Shape

Inside Hair: A Closer Look at Color and Shape For the past decade women and men alike have had chemical treatments preformed on their hair. Consumers spend millions of dollars on hair care products such

### Impacts of Tunnelling on Ground and Groundwater and Control Measures Part 1: Estimation Methods

Impacts of Tunnelling on Ground and Groundwater and Control Measures Part 1: Estimation Methods Steve Macklin Principal Engineering Geologist GHD Melbourne 1. Introduction, scope of Part 1 2. Terminology

### Design of diaphragm and sheet pile walls. D-Sheet Piling. User Manual

Design of diaphragm and sheet pile walls D-Sheet Piling User Manual D-SHEET PILING Design of diaphragm and sheet pile walls User Manual Version: 14.1.34974 31 July 2014 D-SHEET PILING, User Manual Published

### DIELECTRIC SPECTROSCOPY AS A DIAGNOSTIC TEST METHOD FOR THE DETERMINATION OF MECHANICAL DAMAGE IN MARBLE SAMPLES

The 10 th International Conference of the Slovenian Society for Non-Destructive Testing»Application of Contemporary Non-Destructive Testing in Engineering«September 1-3, 2009, Ljubljana, Slovenia, 415-421

### Fundamentals of grain boundaries and grain boundary migration

1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which

### Chapter 8. Low energy ion scattering study of Fe 4 N on Cu(100)

Low energy ion scattering study of 4 on Cu(1) Chapter 8. Low energy ion scattering study of 4 on Cu(1) 8.1. Introduction For a better understanding of the reconstructed 4 surfaces one would like to know

### Topology Optimization of Modified Piston, Bridge Structures and Subway Tunnel Problem

Topology Optimization of Modified Piston, Bridge Structures and Subway Tunnel Problem Akash Dhiman 1, Anadi Misra 2 1PG Student, Mechanical Department, College of Technology, GBPUAT Pantnagar, Uttarakhand-

### THE COMPUTATIONAL MODEL OF THE LOAD DISTRIBUTION BETWEEN ELEMENTS IN A PLANETARY ROLLER SCREW

JOURNAL OF THEORETICAL AND APPLIED MECHANICS 52, 3, pp. 699-705, Warsaw 204 THE COMPUTATIONAL MODEL OF THE LOAD DISTRIBUTION BETWEEN ELEMENTS IN A PLANETARY ROLLER SCREW Jan Ryś, Filip Lisowski Cracow

### I. Basic concepts: Buoyancy and Elasticity II. Estimating Tax Elasticity III. From Mechanical Projection to Forecast

Elements of Revenue Forecasting II: the Elasticity Approach and Projections of Revenue Components Fiscal Analysis and Forecasting Workshop Bangkok, Thailand June 16 27, 2014 Joshua Greene Consultant IMF-TAOLAM

### Behaviour of buildings due to tunnel induced subsidence

Behaviour of buildings due to tunnel induced subsidence A thesis submitted to the University of London for the degree of Doctor of Philosophy and for the Diploma of the Imperial College of Science, Technology

### Page 1. 6. Which hydrocarbon is a member of the alkane series? (1) 1. Which is the structural formula of methane? (1) (2) (2) (3) (3) (4) (4)

1. Which is the structural formula of methane? 6. Which hydrocarbon is a member of the alkane series? 7. How many carbon atoms are contained in an ethyl group? 1 3 2 4 2. In the alkane series, each molecule

### RMS Guide for design of concrete pavements in areas of settlement. Version 1.0. Roads and Maritime Services www.rms.nsw.gov.au

Guide for design of concrete pavements in areas of settlement Version 1.0 RMS Guide for design of concrete pavements in areas of settlement Version 1.0 Roads and Maritime Services www.rms.nsw.gov.au Title:

### Environmental Monitoring with Sensors: Hands-on Exercise

Environmental Monitoring with Sensors: Hands-on Exercise Now that you ve seen a few types of sensors, along with some circuits that can be developed to condition their responses, let s spend a bit of time

### FDM Part Quality Manufactured with Ultem*9085

FDM Part Quality Manufactured with Ultem*9085 A. Bagsik 1,2, V. Schöppner 1, E. Klemp 2 1 Kunststofftechnik Paderborn (KTP),Universität Paderborn, D-33102 Paderborn, Germany 2 Direct Manufacturing Research

### Symmetric Stretch: allows molecule to move through space

BACKGROUND INFORMATION Infrared Spectroscopy Before introducing the subject of IR spectroscopy, we must first review some aspects of the electromagnetic spectrum. The electromagnetic spectrum is composed

### Subminiature Load Cell Model 8417

w Technical Product Information Subminiature Load Cell 1. Introduction... 2 2. Preparing for use... 2 2.1 Unpacking... 2 2.2 Using the instrument for the first time... 2 2.3 Grounding and potential connection...

### APPENDIX G SETTLEMENT

APPENDIX G SETTLEMENT TABLE OF CONTENTS G.1 IN T R O D U C T IO N... 1 G.2 MATERIAL PLACEMENT AND COMPACTION... 1 G.2.1 Incom pressible M aterials... 1 G.2.2 Compressible Materials... 2 G.2.3 Soil P lacem

### Finite Element Analysis of Elastic Settlement of Spreadfootings Founded in Soil

Finite Element Analysis of Elastic Settlement of Spreadfootings Founded in Soil Jae H. Chung, Ph.D. Bid Bridge Software Institute t University of Florida, Gainesville, FL, USA Content 1. Background 2.

### For example, estimate the population of the United States as 3 times 10⁸ and the

CCSS: Mathematics The Number System CCSS: Grade 8 8.NS.A. Know that there are numbers that are not rational, and approximate them by rational numbers. 8.NS.A.1. Understand informally that every number

### EUROPEAN ORGANISATION FOR TECHNICAL APPROVALS

E TA TECHNICAL REPORT Design of Bonded Anchors TR 29 Edition June 27 EUROPEAN ORGANISATION FOR TECHNICAL APPROVALS TABLE OF CONTENTS Design method for bonded anchors Introduction..4 1 Scope...2 1.1 Type

### Where Is My Lone Pair?

Where Is My Lone Pair? Goal: In this tutorial we'll learn how to determine which orbital contains a lone pair. This is important for resonance, conjugation, and aromaticity. To master this subject you'll

### TECHNICAL INFORMATION

TECHNICAL INFORMATION ANALYSIS OF SOLID TANTALUM CAPACITOR LEAKAGE CURRENT by R. W. Franklin AVX Long Road Paignton Devon TQ4 7ER Abstract: The leakage current of a solid tantalum capacitor is the sum

### ! # # % % & () +, & +,,. / 0 % 1 + + 0 % 1 + + 2) () 3

! # # % % & () +, & +,,. / 0 % 1 + + 0 % 1 + + 2) () 3 4 SEISMIC EVALUATION OF REDUCED WEB SECTION(RWS) MOMENT CONNECTIONS Konstantinos Daniel Tsavdaridis Assistant Professor of Structural Engineering

### A case study of large screw pile groups behaviour

Jongerenforum Geotechniek 5 juni 2015 A case study of large screw pile groups behaviour Alice Manzotti Content of the presentation 2 Introduction General soil conditions at the site Foundation design -

### Part-Based Recognition

Part-Based Recognition Benedict Brown CS597D, Fall 2003 Princeton University CS 597D, Part-Based Recognition p. 1/32 Introduction Many objects are made up of parts It s presumably easier to identify simple

### Florida Math for College Readiness

Core Florida Math for College Readiness Florida Math for College Readiness provides a fourth-year math curriculum focused on developing the mastery of skills identified as critical to postsecondary readiness

### Lecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip --- the probe.

Lecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip --- the probe. Brief Overview of STM Inventors of STM The Nobel Prize in Physics 1986 Nobel

### White Dwarf Properties and the Degenerate Electron Gas

White Dwarf Properties and the Degenerate Electron Gas Nicholas Rowell April 10, 2008 Contents 1 Introduction 2 1.1 Discovery....................................... 2 1.2 Survey Techniques..................................

### Multiobjective Robust Design Optimization of a docked ligand

Multiobjective Robust Design Optimization of a docked ligand Carlo Poloni,, Universitaʼ di Trieste Danilo Di Stefano, ESTECO srl Design Process DESIGN ANALYSIS MODEL Dynamic Analysis Logistics & Field

### VERILAST Technology for Hip Replacement Implants

VERILAST Technology for Hip Replacement Implants Surgeon Name Clinic Name Clinic Address Clinic i Address Phone Number Web Address Total Hip Replacement What Is VERILAST Hip Technology? OXINIUM Oxidized

### A) F = k x B) F = k C) F = x k D) F = x + k E) None of these.

CT16-1 Which of the following is necessary to make an object oscillate? i. a stable equilibrium ii. little or no friction iii. a disturbance A: i only B: ii only C: iii only D: i and iii E: All three Answer:

### Lecture 6 - Boundary Conditions. Applied Computational Fluid Dynamics

Lecture 6 - Boundary Conditions Applied Computational Fluid Dynamics Instructor: André Bakker http://www.bakker.org André Bakker (2002-2006) Fluent Inc. (2002) 1 Outline Overview. Inlet and outlet boundaries.

### Corrugated Tubular Heat Exchangers

Corrugated Tubular Heat Exchangers HEAT EXCHANGERS for the 21st CENTURY Corrugated Tubular Heat Exchangers (CTHE) Corrugated Tube Heat Exchangers are shell and tube heat exchangers which use corrugated

### Functional Data Analysis of MALDI TOF Protein Spectra

Functional Data Analysis of MALDI TOF Protein Spectra Dean Billheimer dean.billheimer@vanderbilt.edu. Department of Biostatistics Vanderbilt University Vanderbilt Ingram Cancer Center FDA for MALDI TOF

### Lectures 2 & 3. If the base pair is imbedded in a helix, then there are several more angular attributes of the base pair that we must consider:

Lectures 2 & 3 Patterns of base-base hydrogen bonds-characteristics of the base pairs How are double helices assembled?? Figure 13 Let us first examine the angular characteristics of base pairs. Figure

### Symmetric planar non collinear relative equilibria for the Lennard Jones potential 3 body problem with two equal masses

Monografías de la Real Academia de Ciencias de Zaragoza. 25: 93 114, (2004). Symmetric planar non collinear relative equilibria for the Lennard Jones potential 3 body problem with two equal masses M. Corbera,

### ( ) where W is work, f(x) is force as a function of distance, and x is distance.

Work by Integration 1. Finding the work required to stretch a spring 2. Finding the work required to wind a wire around a drum 3. Finding the work required to pump liquid from a tank 4. Finding the work

### 2009-12-23 ICS: 93.160. Strengthening retrofitting of reinforced concrete structures by gluing of fibre reinforced polymeric fabrics (FRP fabrics)

36888 ежглеяис тгс йубеямгсеыс (теувос еутеяо) 20091223 ICS: 93160 150114010801:2009 H HELLENIC CHNICAL SPECIFICATION (FRP ) Strengthening retrofitting of reinforced concrete structures by gluing of fibre

### Handheld Shock Control Design Guide

Handheld Shock Control Design Guide Handheld Shock Control Design Guide Cushioning in Handheld Devices: Understanding Impact The Challenge: Protecting Handheld Devices from Cracks The most devastating

### Enrollment Services: Rev 12/11/2012 1

Enrollment Services: Rev 12/11/2012 1 Purpose of This Guide Page 3 CSULB Major Specific Requirements Page 4 Using ASSIST to Determine Course Equivalencies Between CSULB and California Community Colleges

### Sampling the Brillouin-zone:

Sampling the Brillouin-zone: Andreas EICHLER Institut für Materialphysik and Center for Computational Materials Science Universität Wien, Sensengasse 8, A-090 Wien, Austria b-initio ienna ackage imulation

### Darrick Chang ICFO The Institute of Photonic Sciences Barcelona, Spain. April 2, 2014

Darrick Chang ICFO The Institute of Photonic Sciences Barcelona, Spain April 2, 2014 ICFO The Institute of Photonic Sciences 10 minute walk 11 years old 22 Research Groups 300 people Research themes: Quantum

### SOLUTIONS. f x = 6x 2 6xy 24x, f y = 3x 2 6y. To find the critical points, we solve

SOLUTIONS Problem. Find the critical points of the function f(x, y = 2x 3 3x 2 y 2x 2 3y 2 and determine their type i.e. local min/local max/saddle point. Are there any global min/max? Partial derivatives

### Elasticity and mechanical advantage in cables and ropes

IOP PUBLISHING Eur. J. Phys. 8 (007) 715 77 EUROPEAN JOURNAL OF PHYSICS doi:10.1088/0143-0807/8/4/011 Elasticity and mechanical advantage in cables and ropes MJO Shea Department of Physics, Kansas State

### Study of Analysis System for Bridge Test

Study of Analysis System for Bridge Test Chen Ke, Lu Jian-Ming, Research Institute of Highway, 100088, Beijing, China (chenkezi@163.com, lujianming@263.net) Summary Analysis System for Bridge Test (Chinese

FP7 NMP/INCO Brokerage Event Warsaw, 17-18 September 2009 Dr Marcin Adamiak marcin.adamiak adamiak@polsl.pl http://www.imiib.polsl.pl www.imiib.polsl.pl/ Institute of Engineering Materials and Biomaterials

### 11. Analysis of Case-control Studies Logistic Regression

Research methods II 113 11. Analysis of Case-control Studies Logistic Regression This chapter builds upon and further develops the concepts and strategies described in Ch.6 of Mother and Child Health:

### Iwaki America Is proud to offer the highest value, sealless, non-metallic mag-drive pumps for your chemical process applications. Iwaki America pumps

Iwaki America Is proud to offer the highest value, sealless, non-metallic mag-drive pumps for your chemical process applications. Iwaki America pumps are manufactured solely with nonmetallic wetted parts

### STRENGTH AND DUCTILITY OF WELDED JOINTS SUBJECTED TO OUT OF PLANE BENDING

STRENGTH AND DUCTILITY OF WELDED JOINTS SUBJECTED TO OUT OF PLANE BENDING by Ivan Gomez Amit Kanvinde University of California, Davis Yu Kay Kwan Gilbert Grondin University of Alberta Final Report Presented

### This week. CENG 732 Computer Animation. Challenges in Human Modeling. Basic Arm Model

CENG 732 Computer Animation Spring 2006-2007 Week 8 Modeling and Animating Articulated Figures: Modeling the Arm, Walking, Facial Animation This week Modeling the arm Different joint structures Walking

### Neue Entwicklungen in LS-OPT/Topology - Ausblick auf Version 2

Neue Entwicklungen in LS-OPT/Topology - Ausblick auf Version 2 Willem Roux**, Heiner Muellerschoen*, Katharina Witowski* *DYNAmore GmbH **LSTC contact: hm@dynamore.de DYNAmore GmbH Germany http://www.dynamore.de

### Polymer Termination. Mechanical Cracking 2. The reason for polymer termination. What is Polymer Termination? 3

Polymer Termination An alternative termination material specifically designed to absorb greater levels of mechanical stress thereby reducing capacitor failures associated with mechanical cracking Mechanical

### OPERE DI PROTEZIONE CONTRO LA CADUTA MASSI: ASPETTI PROGETTUALI. Reti in aderenza. Daniele PEILA. Daniele PEILA

OPERE DI PROTEZIONE CONTRO LA CADUTA MASSI: ASPETTI PROGETTUALI Reti in aderenza 0 Simple mesh drapery system 1 Simple mesh drapery system 2 Fixed drapery sistem 3 Fixed drapery sistem 4 Fixed drapery

### Electronic Transport in Ropes of Single Wall Carbon Nanotubes

Electronic Transport in Ropes of Single Wall Carbon Nanotubes Von der Fakultät für Mathematik, Informatik und Naturwissenschaften der Rheinisch-Westfälischen Technischen Hochschule Aachen zur Erlangung

### The CVD diamond booklet

available at: www.diamond-materials.com/download Content 1. General properties of diamond... 2 2. Optical Properties... 4 Optical transparency...4 Absorption coefficient at 10.6 µm...5 Refractive index:

### 4.3 Least Squares Approximations

18 Chapter. Orthogonality.3 Least Squares Approximations It often happens that Ax D b has no solution. The usual reason is: too many equations. The matrix has more rows than columns. There are more equations

### College Readiness Math MOOC

College Readiness Math MOOC Instructor Information: Dr. Jennifer Kosiak, jkosiak@uwlax.edu General email: mathmooc@uwlax.edu Mathematics Department, University of Wisconsin- La Crosse Description: The